In-Vitro Evaluation of the Effect of Herbal Antioxidants on Shear
Bond Strength of Composite Resin to Bleached Enamel
Zahra Khamverdi 1, Parvin Khadem 2, Aliraza Soltanian 3, Maryam Azizi4
1 Professor, Dental Research Center, Department of Operative Dentistry, Faculty of Dentistry, Hamadan University of Medical Sci ences,
2 Assistant Professor, Department of Operative Dentistry, Faculty of Dentistry, Khorasgan Azad University, Isfahan, Iran 3 Associate Professor, Department of Biostatistics, Faculty of Health, Hamadan University of Medical Sciences, Hamadan, Iran 4 Dentist, Hamadan, Iran
Objectives: A reduction in bond strength of composite to bleached enamel has been reported immediately after bleaching treatment. Application of some antioxidant agents may decrease the adverse effects of whitening agents on bond strength and enhance composite bond to enamel. This study aimed to assess the effect of green tea, sodium ascorbate, sage and grape seed extract on bond strength of composite to bleached enamel.
Materials and Methods: In this in-vitro study, 90 human enamel surfaces were randomly divided into six groups as follows (n=15): G1, no bleaching; G2, bleaching with 40% hydrogen peroxide (HP); G3, HP+1000 μmol epigallocatechin gallate (EGCG) for 10 minutes; G4, HP+10% sodium ascorbate for 10 minutes; G5, HP+10% sage for 10 minutes and G6, HP+5% grape seed extract for 10 minutes. The specimens were bonded to composite in all groups. The shear bond strength of specimens was measured in Megapascals (MPa). Data were analyzed using one-way ANOVA and Tukey’s HSD test (α=0.05).
Results: The highest and the lowest mean shear bond strength values were observed in group 1 (22.61±3.29MPa) and group 2 (5.87±1.80MPa), respectively. The reduction in bond strength in group 2 was greater than that in other groups (P<0.001). No significant difference was found among groups 1, 3, 4, 5 and 6 (P>0.05).
Conclusions: All the herbal antioxidants used in this study equally compensated for the reduced bond strength of composite to bleached enamel.
Keywords: Antioxidants; Tooth Bleaching; Composite Resins; Shear Strength
Journal of Dentistry, Tehran University of Medical Sciences, Tehran, Iran (2016; Vol. 13, No. 4)
P. Khadem, Department of Operative Dentistry, Faculty of
Dentistry, Khorasgan Azad
University, Isfahan, Iran
Received: 19 January 2016 Accepted: 2 April 2016
Demand for esthetic dental restorations has significantly increased. Patients pay more attention to smile esthetics and their appearance
than before. Thus, treatment of tooth
discolorations has become increasingly popular . Bleaching is the most commonly used technique for treatment of discolored teeth.
Bleaching agents often contain variable
concentrations of carbamide peroxide or hydrogen peroxide (HP) [2,3].
Increased microleakage of composite
restorations is one side effect of bleaching treatments, which occurs due to the presence of peroxide and free radicals of oxygen. These free radicals interfere with resin polymerization and inhibit the function of adhesive systems . This
inhibitory effect decreases over time.
Researchers recommend postponing the
[13-17], one study showed that sodium ascorbate had the potential of forming a three-dimensional, porous physical scaffold that would entrap the pathogenic microorganisms like Streptococcus mutans and this adverse property affected its efficacy for enhancing the bond strength and highlighted the need for other antioxidants . Grape seed as an herbal antioxidant contains pro-antioxidant compounds and is capable of eliminating free radicals . Studies have shown that polyphenols present in green tea are rapidly metabolized and show antioxidant activity [19,20]. Catechins present in green tea such as epigallocatechin gallate (EGCG) are antioxidant compounds that can eliminate free radicals as well . Sage extract also has antioxidant capacity . Previous studies have shown that these herbal antioxidants can reverse the decreased bond strength of composite to bleached enamel [17,22,23]. However, some studies have reported different efficacy values for herbal products in various application times [24-28]. Also, a large number of studies have compared only one or two herbal antioxidants with sodium ascorbate [23,26,27]. In order to better assess the efficacy of herbal and chemical antioxidants, this in-vitro study was carried out to assess the effect of sodium ascorbate, grape seed, sage and green tea extracts on the bond strength of composite to bleached enamel.
MATERIALS AND METHODS
In this in vitro experimental study, 90 maxillary anterior teeth extracted within the past three months were selected. The teeth were evaluated
under a stereomicroscope at ×7 magnification to
ensure absence of cracks, caries or restorations. The teeth were cleaned using a periodontal curette and immersed in 10% formalin solution (Shahid Ghazi Co., Tabriz, Iran) at room temperature for one week. The teeth were stored
in distilled water (Shahid Ghazi Co., Tabriz,
Iran) 24 hours prior to the experiment. To prepare the specimens, the roots were cut at the
cementoenamel junction using a diamond bur (≠878-016M, SS White Inc., Lakewood, USA) and high-speed handpiece under water and air spray. The pulp tissue was removed by an excavator and the cavity was filled with composite resin (Filtek Z250, 3M ESPE, St. Paul, MN, USA). The labial surface of the teeth was polished with 400 and 600 grit silicon carbide papers, respectively to obtain a smooth, uniform enamel surface in all specimens. Then, the teeth were randomly divided into six groups as follows
G1: No bleaching (control group), G2: Bleaching with 40% HP gel,
G3: Bleaching with HP followed by 1000μmol EGCG solution for 10 minutes,
G4: Bleaching with HP followed by 10% sodium ascorbate solution for 10 minutes,
G5: Bleaching with HP followed by 10% sage solution for 10 minutes, and
G6: Bleaching with HP followed by 5% grape seed extract for 10 minutes.
an Erlenmeyer flask; 20mL of distilled water was added to dissolve the powder. The mixture was placed on a shaker (Unimax 2010, Heidolph, Wetzlar, Germany). The homogenous mixture was filtered using a 0.5mm filter paper (Whatman, Sigma Aldrich Co., St. Louis, USA). Distilled water was added to reach a volume of 100mL in order to obtain 5% grape seed solution . To prepare 1000μmol solution of EGCG, 95% EGCG powder (Sigma Aldrich Co., St. Louis, USA) was dissolved in distilled water. For preparation of 10% sodium ascorbate, 10mg of sodium ascorbate powder was dissolved in 50mL of distilled water and the volume of solution was reached to 100mL . After preparation, all solutions were refrigerated until the experiment.
Bleaching protocol: In groups 2-6, 40% HP (Power Whitening YF White Smile GmbH, Birkenau, Germany) was applied three times to the enamel surfaces for 15 minutes according to the manufacturer’s instructions. The gel was refreshed every 10 minutes. After completion, the specimens were rinsed with water and air spray and air-dried.
Application of antioxidants: Following bleaching, 1000μmol solution of EGCG, 10% sodium ascorbate, 10% sage and 5% grape seed extract were applied to the surface of specimens in groups 3, 4, 5 and 6, respectively for 10 minutes using a microbrush. To compensate for the evaporated solution, the solution applied to the surface was refreshed every one minute. Next, the surfaces were rinsed under running
water and gently air-dried.
Composite resin bonding: To do a composite build-up, 37% phosphoric acid (Ultra etch, Ultra Dent, South Jordan, USA) was applied to the surface of specimens for 30 seconds, rinsed for 15 seconds and dried for 10 seconds. Etch and rinse bonding agent (Single Bond, 3M ESPE, St. Paul, MN, USA) was applied to the specimen surface in two coats with a five-second interval by a microbrush, air dried with air spray for five
seconds and light-cured for 20 seconds from one-millimeter distance using a light curing unit (Hilux LED 550, Benlioglu Dental, Ankara,
Turkey) with a light intensity of 450 mW/cm2.
Clear cylindrical molds (tubes) measuring 4mm in diameter and 5mm in length were placed on
the adhesive-coated surfaces. Light-cure
composite resin (Filtek Z250, 3M ESPE, St. Paul, MN, USA) was incrementally applied in one-millimeter layers. Each layer was cured for 20 seconds from both sides of the clear cylinder. Clear molds were removed by a scalpel and specimens were immersed in distilled water at room temperature for 24 hours to ensure complete polymerization. The shear bond strength was measured using a universal testing machine (Santam, Tehran, Iran) at a crosshead speed of 0.5 mm/minute. Following shear bond strength testing, the fracture surfaces were evaluated under a stereomicroscope (Zoom 2000, Leica Co., Vernon Hills, IL, USA) at x40 magnification. Mode of failure was classified as adhesive (failure at the enamel/composite interface), cohesive (failure in the enamel or composite) and mixed (combination of adhesive and cohesive failures). The data were analyzed with SPSS version 16 (SPSS Inc., IL, USA) using one-way ANOVA and Tukey’s HSD test. Significance level was set at 95% (α=0.05).
The lowest mean bond strength was observed in group 2 (5.87±1.80MPa) and the highest in group 1 (22.61±3.29MPa).
Table 1: Descriptive statistics of bond strength values (MPa) in the six groups (n=15)
Groups Mean (±SD) bond
strength (MPa) Minimum Maximum
1 22.61±3.29 17.50 29.00
2 5.78±1.80 3.40 10.10
3 20.07±1.45 17.80 22.30
4 20.35±2.89 15.50 25.80
5 20.31±2.38 16.80 25.30
6 20.71±2.15 17.60 24.00
Table 1 shows the mean and standard deviation (SD) values of shear bond strength in the six groups studied. One-way ANOVA revealed significant differences in bond strength among the six groups (P<0.001; Table 2).
Table 2: Results of one-way ANOVA
Sum of squares df
square F Sig.
Between groups 2855.792 5 571.158 98.729 .000
Within groups 485.952 84 5.785
Total 3341.744 89
For multiple pairwise comparisons of the groups, the bond strength between group 2 and other groups was significantly different (P<0.001); but no significant difference was found in bond strength between group 1 and groups 3, 4, 5 or 6 (P>0.05). Also, there was no significant difference between groups 3, 4, 5 and 6 (P>0.05; Table 3). The results of mode of failure in the groups using a stereomicroscope are shown in Table 4. Group 2 had the highest frequency of adhesive failure while the mode of failure in other groups was almost similar.
Treatment of bleached teeth is challenging for dentists because they cannot immediately perform a resin restoration on bleached teeth due to the presence of oxygen or peroxide residues on the surface, since they prevent complete polymerization of adhesive resin . However, by postponing the composite restoration for two weeks following bleaching, no reduction in bond strength would occur [5,15,17]. But, sometimes it is not possible for the patient to wait that long. Therefore, use of antioxidants like ascorbic acid or sodium ascorbate is one method to immediately increase the bond strength of composite to bleached enamel [8,10]. It has been proven that application of sodium ascorbate can result in accumulation of Streptococcus mutants on bleached surfaces . Also, pH of sodium ascorbate is 1.8, which has adverse effects on tooth structure in clinical application. Short shelf life of sodium ascorbate solution or gel is another disadvantage of using it [26,27]. It has been demonstrated that use of herbal antioxidants such as green tea and grape seed is an effective alternative strategy for this purpose.
Table 3: Multiple pairwise comparisons of the six groups
Group (I) Group (J) Mean difference (I-J) Standard error Significance
95% Confidence interval
Lower bound Upper bound
2 16.74800* .87827 .000 14.1865 19.3095
3 2.54133 .87827 .053 -.0202 5.1028
4 2.26800 .87827 .113 -.2935 4.8295
5 2.30800 .87827 .102 -.2535 4.8695
6 1.90133 .87827 .265 -.6602 4.4628
3 -14.20667* .87827 .000 -16.7682 -11.6452
4 -14.48000* .87827 .000 -17.0415 -11.9185
5 -14.44000* .87827 .000 -17.0015 -11.8785
6 -14.84667* .87827 .000 -17.4082 -12.2852
4 -.27333 .87827 1.000 -2.8348 2.2882
5 -.23333 .87827 1.000 -2.7948 2.3282
6 -.64000 .87827 .978 -3.2015 1.9215
4 5 .04000 .87827 1.000 -2.5215 2.6015
6 -.36667 .87827 .998 -2.9282 2.1948
5 6 -.40667 .87827 .997 -2.9682 2.1548
Table 4: Fracture mode in the six groups
Group Adhesive N(%)
1 9(60) 2(13) 4(27)
2 14(93) 0(0) 1(7)
3 9(60) 3(20) 3(20)
4 10(57) 2(13) 3(30)
5 9(60) 2(13) 4(27)
6 9(60) 3(20) 3(20)
Several studies have indicated the anticariogenic, antibacterial and antioxidant effects of these herbal extracts [4,6,17]. In addition, herbal products are non-cytotoxic, easily available and affordable with long shelf life. Several studies have indicated that some of these herbal products have antioxidant properties 20 times greater than that of sodium ascorbate [4,29].
In the current study, 1000μmol EGCG, 10% sodium ascorbate, 10% sage and 5% grape seed extract were used because previous studies have demonstrated that these concentrations of the respective compounds can increase the bond strength of composite to bleached enamel to the level of unbleached samples [4,10,17,22,23]. Duration of 10 minutes for the application of antioxidants was selected in the current study according to Turkun and Kaya , Kaya and Turkun , Vidhya et al,  Khamverdi et al,  and Khamverdi and Safari .
Different bleaching agents are used for tooth bleaching depending on the technique. In the current study, 40% HP was used, which is commonly used for in-office bleaching. Some previous studies used other concentrations (10 to 30%) of HP [17,23,30].
The results of the current study showed the lowest bond strength in group 2. Also, significant differences were observed in bond strength between group 2 and other groups. It means that tooth bleaching results in a significant reduction in bond strength.
Reason of this reduction can be related to production of free oxygen radicals in the process of bleaching, which can decrease the bond strength of composite to enamel. Some
researchers indicated a reduction in calcium content of the enamel and a reduction in the enamel surface microhardness, which decrease bond strength [13,18]; while other studies confirmed that oxygen residues create porosities in the enamel surface and negatively affect the bond strength [13,17,20,31]. In the current study, the results showed significant differences in bond strength between group 2 and groups 3-6. These results can be attributed to the antioxidant activity of green tea, sodium ascorbate, sage and grape seed. Lambert and Elias  concluded that EGCG had antioxidant activity. The antioxidant activity of EGCG is due to its chemical formulation and polyphenolic nature. Each molecule of this material includes 4 rings of A, B, C and D. Tri-hydroxyl and di-hydroxyl groups of B ring are believed to be responsible for the
antioxidant property of this material.
Polyphenols inhibit excess generation of reactive oxygen species, increase the degree of polymerization and enhance the bond strength of resin to bleached enamel . Similarly, in our study, green tea increased the bond strength of composite to bleached enamel, which is in line with the results of Khamverdi et al,  and Lambert and Elias . However, Ozelin et al,  indicated that green tea had positive antioxidant effect after 60 minutes; in shorter time periods such as 15 and 30 minutes, it did not increase the bond strength. Moreover, Berger et al,  evaluated the effect of green tea as an antioxidant on bond strength of composite to tooth structure after bleaching for one and six hours and reported that green tea improved the reduced bond strength. Proanthocyanidin is a
plant metabolite containing monomers,
oligomers and catechin polymers. It is commonly found in fruit seeds. Proanthocyanidin has strong antioxidant activity and is capable of eliminating free radicals. In medicine, it is used for its
anti-allergic, antibacterial and anticariogenic
nutritional supplement . Our study also showed the antioxidant activity of grape seed. Its possible mechanism is via the presence of donor sites on oligomeric proanthocyanidin complexes that enhance free radical scavenging and increase the antioxidative effect by esterification of polyphenols in proanthocyanidin complexes . Therefore, it is capable of eliminating free radicals and can increase the bond strength of composite to bleached enamel. This finding was confirmed by Vidhya et al .
Subramonian et al,  reported that herbal products such as pine bark and grape seed extract can compensate for the reduced bond strength of composite to bleached enamel, and pine bark had a greater efficacy than grape seed; the results of our study demonstrated similar antioxidative efficacy of green tea and grape seed, which was in agreement with the results of Sharafeddin et al . However, sage was not evaluated in their study. The current study showed that sage had antioxidant activity and increased the microshear bond strength of composite to bleached enamel. The mechanism of action of sage has yet to be fully understood; however, the antioxidant property of this material is due to its polyphenolic nature and chemical formulation. Polyphenols like caffeic acid, hispidulin, apigenin, rosmanol, carnosic acid, carnosol and ursolic acid are among the active ingredients of sage. Similar to other antioxidants, these polyphenols inhibit the formation of reactive oxygen species [22,34]. This finding was in accord with the results of Khamverdi and Safari . Abraham et al,  compared the antioxidant property of sodium ascorbate and grape seed and concluded that application of grape seed had greater efficacy for reversal of compromised bond strength of composite to bleached enamel; whereas, Arumugam et al,  reported opposite results. It is stated that high molecular weight of proanthocyanidin is an important factor responsible for its less penetration into tooth structure and reducing
oxygen free radicals. The findings of our study showed equal antioxidant efficacy of grape seed and sodium ascorbate, which is in accord with the
results of Vidhya et al,  and Sharafeddinet al,
. Two in-vitro studies demonstrated that grape seed extract inhibited the demineralization and enhanced the remineralization of carious root lesions [4,33]. The results of microscopic analysis confirmed the findings of shear bond strength testing in our study, since group 2 with the lowest bond strength value had the highest frequency of adhesive failure. In the current study, antioxidants were applied in the form of solution. Use of antioxidants in the form of hydrogel is recommended in future studies. In the current study, antioxidants were used for 10 minutes. Other studies are required to assess the effect of higher concentrations of antioxidants with shorter application times. Since antioxidants have a short shelf life, future studies are recommended to focus on the storage methods of antioxidants. The current study had an in-vitro design and clinical studies are needed to further elucidate this issue.
Within the limitations of this study, tooth bleaching significantly decreased the bond strength of composite to enamel. All the herbal antioxidants used in this study equally reversed the reduced bond strength of composite to bleached enamel.
The authors would like to thank Dr. Toliat for solutions preparing and the Dental Research Center and Vice Chancellor of Research, Hamadan University of Medical Sciences, for supporting this study.
1- Kihn PW. Vital tooth whitening. Dent Clin North
Am. 2007 Apr;51(2):319-31.
RV, Botero T, Tarquinio SB. Erosion and abrasion on dental structures undergoing at-home bleaching. Clin Cosmet Investig Dent. 2011 Jul;3:45-52.
3- Minoux M, Serfaty R. Vital tooth bleaching:
biologic adverse effects-a review. Quintessence Int. 2008 Sep;39(8):645-59.
4- Vidhya S, Srinivasulu S, Sujatha M, Mahalaxmi S.
Effect of grape seed extract on the bond strength of bleached enamel. Oper Dent. 2011 Jul-Aug;36(4): 433-8.
5- Algahtani MQ. Tooth bleaching procedures and
their controversial effects: A literature review. Saudi
Dent J. 2014 Apr;26(2):33-46.
6- Turkun M, Kaya AD. Effect of 10% sodium
ascorbate on the shear bond strength of composite resin to bleached bovine enamel. J Oral Rehabil. 2004 Dec;31(12):1184-91.
7- Attin T, Vollmer D, Wiegand A, Attin R, Betke H.
Subsurface micro hardness of enamel and dentin after different external bleaching procedures. Am J Dent. 2005 Feb;18(1):8-12.
8- Kaya AD, Turkun M. Reversal of dentin bonding
to bleached teeth. Oper Dent. 2003 Nov-Dec;28 (6):825-9.
9- Lambert JD, Elias RJ. The antioxidant and pro-oxidant activities of green tea polyphenols: A role in cancer prevention. Arch Biochem Biophys. 2010 Sep;501(1):65-72.
10- Kaya AD, Türkün M, Arici M. Reversal of compromised bonding in bleached enamel using antioxidant gel. Oper Dent. 2008 Jul-Aug;33(4):441-7.
11- Lima AF, Fonseca FM, Freitas MS, Palialol AR, Aguiar FH, Marchi GM. Effect of bleaching treatment and reduced application time of an antioxidant on bond strength to bleached enamel and subjacent dentin. J Adhes Dent. 2011 Dec;13(6):537-42.
12- Nour El-din AK, Miller BH, Griggs JA, Wakefield C. Immediate bonding to bleached enamel. Oper Dent. 2006 Jan-Feb;31(1):106-14.
13- Poorni S, Kumar RA, Shankar P, Indira R, Ramachandran S. Effect of 10% sodium ascorbate on the calcium: Phosphorus ratio of enamel bleached
with 35% hydrogen peroxide: an in vitro quantitative energy-dispersive X-ray analysis. Contemp Clin Dent. 2010 Oct;1(4):223-6.
14- Yun JH, Pang EK, Kim CS, Yoo YJ, Cho KS, Chai JK, et al. Inhibitory of green tea polyphenol on the expression of matrix metalloproteinase-9 and on the formation of osteoclast. J Periodontal Res. 2004 Oct;39(5):300-7.
15- Kato MT, Magalhães AC, Rios D, Hannas AR, Attin T, Buzalaf MA. Protective effect of green tea on dentin erosion and abrasion. J Appl Oral Sci. 2009 Nov-Dec;17(6):560-4.
16- Frei B, Higdon JV. Antioxidant activity of tea polyphenols in vivo: evidence from animal studies. J Nutr. 2003 Oct;133(10):3275S-84S.
17- Khamverdi Z, Rezaei-Soufi L, Kasraei S, Ronasi N, Rostami S. Effect of epigallocatechin gallate on shear bond strength of composite resin to bleached enamel: an in vitro study. Restor Dent Endod. 2013 Nov;38(4):241-7.
18- Kimyai S, Valizadeh H. The effect of hydrogel and solution of sodium ascorbate on bond strength in bleached enamel. Oper Dent. 2006 Jul-Aug;31(4): 496-9.
19- Young IS, Woodside JV. Antioxidants in health and disease. J Clin Pathol. 2001 Mar;54(3):176-86. 20- Dabas D, Patil AC, Uppin VM. Evaluation of the effect of concentration and duration of application of sodium ascorbate hydrogel on the bond strength of composite resin to bleached enamel. J Conserv Dent. 2011 Oct;14(4):356-60.
21- Muraguchi K, Shigenobu S, Suzuki S, Tanaka T. Improvement of bonding to bleached bovine tooth surfaces by ascorbic acid treatment. Dent Mater J. 2007 Nov;26(6):875-81.
22- Khamverdi Z, Safari M. In-vitro evaluation of the effect of sage on shear bond strength of composite resin to bleached enamel. J Islam Dent Assoc Iran 2013 Dec;25(4):366-72.
24- Subramonian R, Mathai V, Christaine Angelo JB, Ravi J. Effect of three different antioxidants on the shear bond strength of composite resin to bleached enamel: An in vitro study. J Conserv Dent. 2015 Mar-Apr;18(2):144-8.
25- Berger SB, De Souza Carreira RP, Guiraldo RD, Lopes MB, Pavan S, Giannini M, et al. Can green tea be used to reverse compromised bond strength after bleaching? Eur J Oral Sci. 2013 Aug;121(4):377-81. 26- Ozelin AA, Guiraldo RD, Carvalho RV, Lopes MB, Berger SB. Effects of green tea application time on bond strength after enamel bleaching. Braz Dent J. 2014 Sep-Oct;25(5):399-403.
27- Abraham S, Ghonmode WN, Saujanya KP, Jaju N, Tambe VH, Yawalikar PP. Effect of grape seed extracts on bond strength of bleached enamel using fifth and seventh generation bonding agents. J Int Oral Health. 2013 Dec;5(6):101-7.
28- Arumugam MT, Nesamani R, Kittappa K, Sanjeev K, Sekar M. Effect of various antioxidants on the shear bond strength of composite resin to bleached enamel: An in vitro study. J Conserv Dent.
29- Fine AM. Oligomeric proanthocyanidin
complexes: history, structure, and phytopharma-ceutical applications. Altern Med Rev. 2000 Apr;5 (2):144-51.
30- Han Y, Mo S, Jiang L, Zhu Y. Effects of antioxidants on the microleakage of composite resin restorations after external tooth bleaching. Eur J Dent. 2014 Apr;8(2):147-53.
31- Bulut H, Turkun M, Kaya AD. Effect of an antioxidizing agent on the shear bond strength of brackets bonded on bleached human enamel. Am J Orthod Dentofacial Orthop. 2006 Feb;129(2):266-72. 32- Kanwar J, Taskeen M, Mohammad I, Huo C, Chan TH, Dou QP. Recent advances on tea polyphenols. Front Biosci (Elite Ed). 2012 Jan;4:111-31.